Lorna Anguilano, Simon Timberlake and Thilo Rehren
ABSTRACT: Excavations in 2002 at Cwmystwyth, in Central Wales, found an ancient lead smelting site. There are remains of the medieval and the Roman periods. This paper describes in brief the excavation of the medieval lead bole (Timberlake 2002a) but also provides an archaeological reconstruction of this and details of an experimental lead smelt carried out at the site in 2003 (by ST). The analytical study (by LA) is of the medi- eval metallurgical debris excavated in 2002, mostly slag, but also ore and lead. The aim was to understand the raw material, the metal produced and the smelting process. The ore smelted was predominantly galena but with no detectable silver, showing it was prob- ably exploited to produce lead. The extremely high sulphur content of the slag indicates that the ore was not roasted before smelting. It is argued that the medieval activity was small-scale, smelting a very rich ore. The furnaces apparently did not require much capital investment, enabling a short-lived and/or exploratory smelting operation.
Background (Level Fawr) Mines, and Copa Hill. Smaller workings abound, such as the Penguelan Mine immediately to Geology and mineralogy the north of Banc Tynddol and the valley road. The The hydrothermal ore veins in the area of Cwmystwyth principal mineralization involves lead and zinc (galena in Central Wales have intermittently sustained a metal and sphalerite) with some copper (chalcopyrite), but production spanning thousands of years, from the Early nickel and antimony are also present in trace amounts. Bronze Age up to the recent past. The whole area is The following minerals have been recorded: galena, intersected by a large system of faults; mineralization sphalerite, chalcopyrite, malachite, marcasite, native occurred along ENE-WSW trending normal faults and copper, pyromorphite, cerussite, hemimorphite, broch- breccia zones that cut across folds of early Devonian age antite, dolomite (ankerite), quartz and linarite (Dobson in Lower Silurian turbidites and sandstones. The normal 1995). faults have 10- to 30m-wide, laterally impersistent, breccia zones. Dating suggests that the mineralization Prehistoric mining occurred in the Upper Palaeozoic (Dobson 1995). The site is best known amongst archaeologists for its prehistoric copper mine, the Comet Lode Opencast, At the Cwmystwyth Mines the main Cwmystwyth the latter exploiting a rich shoot of lead and copper Fault, which post-dates the emplacement of the mineral (chalcopyrite) ore at the point where this vein outcrops lodes, runs parallel to and along the floor of the Upper at 426 metres OD on the side of Copa Hill (Timberlake Ystwyth Valley, and most of the old workings are in 2003; Mighall et al 2000). Abundant stone hammers the hillside to the north of the fault. The fault itself is a and massive spoil heaps containing some 5000 metric conspicuous and major feature of the landscape in that tonnes of prehistoric mine waste bear testimony to the it has influenced the course of the River Ystwyth and its large-scale nature of the operation, whilst archaeological U-shaped glaciated valley. The mineral workings, which excavations carried out here have proved the presence of extend for more than a mile along the north side of the wooden drainage launders, antler tools, withy handles, valley, consist of the Mitchells, Pugh’s and Kingside rope and basketry dating from the Early Bronze Age.
Historical Metallurgy 44(2) 2010 85–103 85 ANGUILANO ET AL: LEAD SMELTING AT CWMYSTWYTH HM 44(2) 2010
The ancient workings here extend to depths of over 10m. What evidence there is to be found within a number Very little, however, is known about the smelting of of brief reports which mention the following types of copper and lead sulphide ores in prehistory. As regards remains: the discovery of small spreads of lead-rich slag copper, the earliest miners at Cwmystwyth could have and charcoal such as those found at Pontrhydygroes been separating and extracting the small amount of (Maen Arthur), Bow Street and Ysbyty Ystwyth (Davies oxidized ores from the sulphides (Timberlake 2009). 1936, 305) and also at Cwm Bwa, Penrhyncoch (Davies 1937; Hughes 1990,13); the discovery of lead metal Early lead mining trapped within cracks or fissures in the rocks such Evidence for Roman and medieval mining for lead is as in the nearby Hafod Estate (Chambers 1858); the beginning to emerge as a result of further archaeological existence of rocky hearths without any upstanding work carried out at these mines and from the palaeo- structures at Hafod; and the discovery of traces of fused pollution record preserved within the blanket peat cover- stone and gritty clay furnace lining alongside other ing the top of Copa Hill (Mighall et al 2002). An ancient refractory materials at Cwm Bwa (Davies 1937, 303). mining leat carrying water from the headwaters of the Such remains are all fairly typical of bole-smelting sites, Nant yr onnen stream to a reservoir within the infilled the use of which is much more likely to have been medi- prehistoric opencast for the purposes of hushing appears eval than post-medieval in date (Tylecote 1986; Willies to have been already abandoned by the 13th century and Cranstone 1992). Moreover, all of these sites are AD, and may be a lot earlier still (Timberlake 2003, close to mines considered on other grounds to be ancient, 13). There are also indications of medieval prospecting Cwmystwyth being no exception (Fig 1). activity within the same area. The earliest clear documentary reference to mining The re-discovery in 1990 of the ‘ancient smelting site’ at Cwmystwyth is that provided by John Leland, the first referred to by the geologist O T Jones in 1921 at King’s Antiquary under Henry VIII who passed along Penguelan (Banc Tynddol) thus provides a link with the valley while on his way from Strata Florida Abbey both this and other circumstantial evidence for early to Llanbadarn sometime between 1536 and 1539. He de- lead mining at Cwmystwyth. scribes what would appear to be contemporary diggings on the Graig Fawr (Fig 2a) plus evidence of former smelting: ‘... I saw on the right hand on a Hill side Cloth- Documentary and field evidence for medieval moyne [Cloth or Clodd = mine, Moyne or Mwyn = lead, smelting perhaps a reference to ‘Craggie-Moyne’, or Graig Fawr], Prior to 1560, though poorly documented, lead and where hath been greate digging for lead the melting silver mining in north Ceredigion was most probably whereof hath destroid the Woddes that sometime grew small-scale and quite underdeveloped compared with plentifull thereabout ...’ (Meyrick 1907, 140). Although that of Flintshire, the majority of mines being little the locations of these offending smelting hearths cannot more than near-surface trials or opencast rakes ex- be deduced from this account, the tree-loss he describes ploited intermittently as local demand for lead rose and is most likely to have taken place on the lower, less steep fell. Typically, lead would have been in demand for slopes of the valley and valley floor, the slightly more the upkeep of castles, an example being the repair of elevated parts of which would have been suitable for Cardigan Castle carried out using lead from the Strata the furnace sites. Florida Mines in 1451 (Lewis 1967), and for the con- struction and repair of churches and abbeys such as Today most of the area along this part of the valley side the Cistercian house of Strata Florida (Hughes 1981) a is covered with either river gravel, mine spoil, scree, or little over 10km south of Cwmystwyth. The presence else cuttings and embankments for the tramroads and of two inspectors of silver at Cardigan in 1340 might leats, thus it is little surprise that no evidence for these suggest the mining of argentiferous ore and also some hearths have (until now) come to light. However, one small-scale production of silver coinage (Lewis 1967) clue as to the possible location of one of these sites was whilst at Strata Florida there are claims that the monks to be found on a map of the mineral veins and workings were practising cupellation (Williams 1889). on Copa Hill published by the geologist Professor O T Jones (1921) which refers to the ‘Remains of Ancient There are few references to lead smelting within the Lead Smelting Works’ at Penguelan (Fig 2a). However, Upper Ystwyth Valley, yet this situation is not that the poor description of this plus the absence of any ob- different from that encountered elsewhere in the north vious surface evidence meant that all previous searches Ceredigion mining field in the period leading up to 1500. had failed to locate it (Hughes 1981).
86 HM 44(2) 2010 ANGUILANO ET AL: LEAD SMELTING AT CWMYSTWYTH
Figure 1: Suggested sites of medieval lead mining and smelting in north Ceredigion.
Our attention was first drawn to this site (SN 809748) and 12 were dug during 2002/3 (Fig 2c). Trenches 10 during the course of a detailed landscape survey of Copa and 12 uncovered the course of an 8m-long channel of Hill carried out by the Early Mines Research Group in lead spill downslope of the Roman hearth in PSS4. The 1989–1990. An area of pronounced infertility amplified latter was excavated in 2002 but is not discussed in any by the dry summer conditions could clearly be seen on detail here as this paper focuses on the bole hearths the rough pastureland which covers a lobe of glacial found in Trench 6 and the smelting remains found in outwash moraine at Banc Tynddol some 30–40m above both Trenches 5 and 6. the valley road. During fieldwalking, small fragments of burnt and pitted rock with the occasional fragment of Geochemical and geophysical surveys fused galena attached were picked up from amongst the In 1996 a soils geochemical survey was undertaken of shallow sheep-disturbed soils, confirming the presence of a 25m2 plot within the area of presumed smelting ac- one or more destroyed hearths (Timberlake 1990, 9). tivity using a portable XRF analyser (Spectrace 9000). This revealed a generally high level of contamination of Excavation of the Banc Tynddol lead around 5000ppm lead, but with hot-spot anomalies of smelting site (ST) up to 25,000ppm (2.5% Pb) (Fig 2d). Elevated levels of potassium here may be linked to the presence of charcoal Following geochemical and geophysical surveys, ar- and ash in the soil (Jenkins and Timberlake 1997, 29). chaeological evaluation of the site took place in 1999, 2002 and 2003. Sample trenches (test pits) PSS1, 2 A larger area (625m2) including both the western and and 3 were dug in 1999, while trenches PSS4–6, 10 eastern ridges of the plateau was geophysically surveyed
87 ANGUILANO ET AL: LEAD SMELTING AT CWMYSTWYTH HM 44(2) 2010
Figure 2: a) Location map of Cwmystwyth – mines and smelting site; b) geophysical survey of Banc Tynddol – magnetic susceptibility and electrical conductivity anomaly map (Archaeophysica Ltd 1999); c) Banc Tynddol plateau and Penguelan Mine, Cwmystwyth showing areas of excavation, survey and experiment; d) geochemical anomaly maps of soil contamination at Banc Tynddol (after Jenkins and Timberlake 1997).
88 HM 44(2) 2010 ANGUILANO ET AL: LEAD SMELTING AT CWMYSTWYTH by Archaeophysica Ltd in June 1999 prior to the first investigation focused on another geophysical anomaly sample excavations. Volumetric magnetic susceptibility (PSS4) located c15m downslope, on the west flank of and electrical conductivity contour surveys revealed the easternmost ridge of the plateau (Fig 2c). very similar positive anomaly patterns suggesting the presence of a number of well-localised areas of strong Early medieval bole hearths burning (or spreads of burnt rock and slag), perhaps In contrast with the pit bole hearth (in PSS4), the bole equating to between five and seven hearths (Fig 2b). The sites (in PSS5 and PSS6) showed almost no evidence east-west orientation of these anomalies, located along for any sub-surface component, whether a trench, pit, the crests of the two ridges, suggested to us that these post-holes or even any sort of credible stone foundation. might well be wind-blown furnaces. Moreover, the archaeology here was thin, a maximum of 150–200mm above a natural (?) spread of boulders Archaeological evaluation  (Fig 3b). The latter had been subjected to a fair In 1999 three 4m2 sample trenches were opened up within degree of erosion as well as modern disturbance along the above area to investigate some of the anomalies and its upper edge. Nevertheless, the record for the exist- possible hearth sites identified (Fig 2c). The westernmost ence of these boles was clearly evident in the form of trench (PSS1), located on the margins of the surveyed in situ burning, and overlying this a layer of charcoal area, uncovered a patch of disturbed ground with burnt and earth  and heat-decrepitated rock [006b]. An stone, slag and 18th–19th century bottle glass at a depth additional scatter of glassy slag, part-fused and unfused of between 100–200mm. However, beneath this lay a galena, melted masses of metal and sulphide (including thick layer of charcoal and ash which appeared to be in lead ‘matte’), plus the occasional droplet of melted lead situ and associated with localised burning of the under- covered the site. At least some of these appeared to have lying ground surface. The absence of any fused lead been formed in situ, the metal having dropped or flowed ore or slag here was considered to be significant, thus down cracks in between the boulders. These suggest the this was originally interpreted as being the remains of a presence of elevated bole sites constructed above ground, possible charcoal clamp or oven, although on reflection much of the stone fabric of which, such as the dry-stone this could just have been the raked out embers of a large (shale) walling surround, appears to have completely hearth(s). A date of 820 ± 60 yrs BP (1030–1300 Cal AD disintegrated on firing. at 95% probability; Beta-140992) was obtained from a bulk sample consisting of small pieces of Quercus sp The bases of at least two boles (A and B) can be identified (oak) charcoal (Timberlake 2002a, 49). This provided within trench PSS6 (Fig 3a), the centres of which ap- the first indication of the period of the site, suggesting pear to have been raked clean (in fact much of the burnt that we were looking at a phase of smelting activity earth and charcoal may have been scraped away in the contemporary with the building and early occupation process of recovering any residual smelted lead metal of the Cistercian Abbey of Strata Florida. This was a and un-smelted/part-smelted ore and lead-rich slags logical conclusion, given that we were well aware of the for re-smelting). It appears that some of the upstanding circumstantial and later documentary evidence that the earth-fast boulders here may also have been selected monks had mining interests at Cwmystwyth (Meyrick as foundations for the building of boles. Many of these 1907, 567; Hughes 1981, 7). are only very lightly burnt, suggesting the presence of a thick covering of turf at the time smelting commenced. The two other trenches (PSS2 and PSS3) were located Some evidence of the quarrying of the underlying on the ridge crests, much closer to the area we now know boulder layer  for the purposes of bole construction to be the focus of bole hearth construction. No actual is evident within a number of areas. Moreover there is hearths were identified at the specific locations cor- some suggestion that the putative grave located beneath responding to the anomalies, but considerable spreads the find of the Beaker gold foil disc (Timberlake 2002b; of raked-out burnt rock, part-fused ore and slag were 2004, 137) was disinterred, then heavily robbed of stone recovered, along with small droplets and runnels of lead by the medieval smelters. For this reason it may now be metal. This appeared to confirm that we were looking at very difficult to recognize the remains of any eroded or the remains of lead–smelting hearths. flat cairn once present at this spot.
Excavation of the bole hearth sites Important information has, however, been forthcom- In October 2002 larger excavation trenches (PSS5 and ing from the dating of charcoal linked to the use of PSS6) were opened up in the area identified above as these boles. A radiocarbon date of 1060 ± 40 yrs BP being the centre of the bole site. Meanwhile a separate (880–1020 Cal AD at 95% probability; Beta-181060)
89 ANGUILANO ET AL: LEAD SMELTING AT CWMYSTWYTH HM 44(2) 2010
b Figure 3: Banc Tynddol Site PSS6. a) plan of trench at the level of 006 (base of boles); b) Section 3, the bole destruction layers; c) lump of melted lead with adhering charcoal found in between boulders on edge of bole A.
was obtained from charcoal pieces associated with the a crude estimate of the total amount of lead smelting lump of melted lead recovered from the ‘channel’ around which has taken place can still be made. Somewhat less the edge of bole A (Fig 3c). Given that this charcoal than 20 tonnes of slag, part-smelted ore and burnt rock was of branchwood, the sample date provided above waste probably cover the entire area of the Banc Tynddol would realistically seem to suggest a date earlier than plateau, whilst the geophysical evidence for areas of the Cistercian interest in the mine as the Abbey of Strata burning (within the surveyed area) suggests the presence Florida was founded in 1164 AD (Hughes 1981, 5). of between 6–10 furnace sites over the whole site. Some Meanwhile, another radiocarbon date of 1264 ± 27 yrs of these, of course, may be earlier or later in date. BP (670–840 Cal AD at 95% probability; OxA-12956) was obtained from a single small piece of oak charcoal Even if this activity amounted to the smelting of recovered during excavations carried out on the bole site 50–100 tonnes of ore, this would still represent only a and grave in 2003 (Timberlake 2004, 137). This adds very small part of the total production from medieval weight to the suggestion that what we are in fact looking mining prior to AD 1500 (Hughes 1981, 6). The scale at is the repeated use of the same bole location for small- of activity here would also not account for the level scale lead smelting over a 300–400 year period. of environmental destruction witnessed by Leland as being evident in 1539. Discussion The amount of surface disturbance and erosion here Other evidence to consider here are those rises in makes it quite difficult now to accurately locate the boles atmospheric lead pollution recorded within the om- or else to quantify the scale of activity. Nevertheless, brotrophic blanket peat on Copa Hill and ascribed to
90 HM 44(2) 2010 ANGUILANO ET AL: LEAD SMELTING AT CWMYSTWYTH
Left to right, Figure 4: Slag sample from trench 5, width 60mm. Figure 5: Furnace wall associated with slag from trench 6, width 66mm. Figure 6: Galena sample from trench 6, width 46mm. early medieval mining (Mighall et al 2002, 181). It Analyses of medieval lead slag from the is true that these tend to be small (typically less than Banc Tynddol excavations (LA) 50ppm lead recorded at depths of between 400 and 200mm in cores CH1, 2 and 4), in particular when During the excavations, described above, various compared with the lead peaks of up to 60ppm lead metallurgical materials were recovered, namely slag linked to Roman working. Nevertheless, it should be sensu stricto, furnace walls associated with slag, lead remembered that the smelting sites at Banc Tynddol metal, galena (unreacted or semi-reacted) and a fragment are some distance from the top of Copa Hill, also that of iron metal. All the materials of interest were found the epicentres of Roman and early-medieval mining in two layers associated with a high concentration of activity at Cwmystwyth may be quite different (this ash and charcoal, close to where the sites of the bole is something which could quite easily be established hearths A and B were identified within the excavations through the analysis of ores from the two different (Fig 3a). types of smelting hearth). Furthermore, the pollution peaks themselves need to be properly dated. The material can be grouped into four different categories: In conclusion, it seems that one of the areas of wind- Slag: several kilograms of slag were excavated from an powered lead smelting located on the valley floor has area of about 16m2. Most fragments are broken, with been identified, and some insight into the different maximum dimension of 40–50mm. The slag pieces are types of bole constructed, the period(s) of their use, covered by a white to red corrosion patina typically 1mm and the approximate number of furnaces/quantities of thick (Fig 4). The density of several pieces was found ore processed have been gained. The archaeological to be 5–6g/cm3, clearly higher than fayalitic copper or evidence so far supports what little is known from iron slag which is 3–4g/cm3. documentary accounts of mining and smelting, as Furnace wall material: burnt stone associated with well as from the environmental record (peat bog slag; the surfaces are blackened by fire and covered by archive) as regards local lead pollution. However, a brown-red patina (Fig 5). These are the majority of the there remain a number of important questions. Who metallurgical remains found at the site. was carrying out mining and smelting here prior to the Lead metal: drops or fragments, some with the typical peak demands for lead brought about by the creation shape of runnels, and some associated with the ex- of the Cistercian houses and lands? Were the small- cavation of a ‘channel’ (possibly a former animal hole) scale smelting campaigns witnessed at Banc Tynddol less than a metre from the furnace (Fig 3c). representative of what were in effect little more than Galena: several fragments of unreacted or semi-reacted occasional bouts of mining, or were there more im- galena, with a deep white alteration patina (Fig 6). The portant bole sites located elsewhere upon the floor and samples are often associated with quartz fragments. sides of this valley? If so, was the smelting at Banc Tynddol simply ‘experimental’, carried out as a means Analytical methods to assay the ore and metal from a variety of different The study involved the use of three analytical veins and workings? methods: optical microscopy (OM), energy dispersive X-ray fluorescence spectrometry (ED-XRF), and
91 ANGUILANO ET AL: LEAD SMELTING AT CWMYSTWYTH HM 44(2) 2010
Table 1: Composition of the glass matrix in the slag samples (wt%).
Sample SiO2 Al2O3 FeO CaO K2O PbO ZnO 5-4b 18.9 1.5 1.8 0.8 0.5 71.6 4.6 5-4c 33.9 2.9 1.7 1.2 1.5 54.6 4.3 5-4e 20.4 1.8 1.6 1.0 0.6 70.5 4.1 6B-2b-a 19.9 1.9 1.5 0.9 0.3 71.6 4.0 6B-2b-c 21.4 1.8 1.7 1.0 0.4 69.1 4.1 6B-2b-d 17.7 1.6 1.1 0.7 0.5 75.9 2.5
Table 2: Bulk slag composition (wt% XRF analysis).
Sample SiO2 Al2O3 Fe2O3 CaO BaO Na2O K2O MnO MgO PbO CuO Sb As2O3 Ag S ZnO % % % % ppm % % % % % ppm ppm ppm ppm % % 5-4a 16.8 1.34 1.03 0.64 103 nd 0.12 0.02 nd 74.8 207 1051 528 16 3.11 2.12 5-4b 16.5 1.00 1.17 0.62 79 nd 0.16 0.02 nd 75.1 61 704 480 11 3.32 2.12 5-4c 20.6 1.50 1.24 0.74 158 nd 0.27 0.02 0.07 70.4 116 1028 669 13 2.38 2.77 5-4e 16.9 1.78 1.16 0.58 105 nd 0.13 0.01 nd 74.8 221 1114 350 19 2.47 2.12 6b-2b-a 13.8 0.96 0.72 0.52 95 1.40 0.07 0.01 nd 76.7 136 1381 375 nd 4.50 1.24 6b-2b-b 17.9 1.25 1.31 0.59 112 nd 0.25 0.02 0.09 72.7 131 617 533 nd 2.71 3.17 6b-2b-d 16.4 1.48 1.07 0.59 114 nd 0.14 0.02 nd 75.4 224 1022 390 14 2.86 2.04 6b-2b-f 17.0 1.08 1.32 0.29 91 nd 0.11 0.02 nd 73.6 133 592 198 9 2.94 3.63 6b-2b-o 14.0 1.11 0.93 0.62 98 nd 0.12 0.02 nd 77.6 147 1391 548 14 4.13 1.40 6b-2b-q 15.2 1.31 1.00 0.70 101 0.86 0.10 0.02 nd 76.0 146 1523 678 21 3.40 1.40
Note: Sample numbers starting 5- are from trench PSS5 and those starting 6b- are from trench PSS6. scanning electron microscopy with energy dispersive ing standard metallographic procedures. For ED-XRF the spectrometry (SEM-EDS). samples were prepared as powder pellets after grinding to less than 1.25µm in a rotation mill with an agate set. Lead is a challenging element for energy dispersive in- The SEM-EDS analyses were either spot analyses of the struments as the high lead concentration in the samples crystals (sulphides and silicates) to establish their com- results in a high absorption of characteristic X-rays of position, or area analyses of the glassy matrix, avoiding lighter elements due to high mass attenuation. For the the sulphide inclusions, in order to selectively determine XRF analyses a generic calibration curve set up for ox- the composition of the liquid phase. Five area analyses ides was used; a calibration curve for lead-rich materials were performed on different areas of the sample to show is under development, but was not yet available for this their chemical homogeneity/non-homogeneity. The data research. The SEM-EDS analyses are based on a ZAF is given in Table 1 and graphically presented in Figures correction procedure and were tested for their accuracy 13 and 14 (see below). by analysing known lead-rich phases; the results for lead sulphide were within a few percent relative to Results the ideal stoichiometric composition, indicating that Thirteen samples were analysed, including eleven slags there are no major analytical problems with the major (see Tables 1 and 2), one ore sample (6B-2b-g) and one components in these compositionally relatively simple furnace wall fragment (4-3/04a). systems. However, minor and trace element data may be less accurate for both instruments. The furnace wall stones with slag adhering to them (eg Fig 5) show no alteration by the smelting process, such The samples were prepared for the microscopes follow- as traces of burning or newly-formed high-temperature
Table 3: Major element composition of the furnace wall (wt% XRF analysis).
Sample SiO2 Al2O3 Fe2O3 Na2O K2O PbO CaO TiO2 MgO ZnO 4-3/04a 64.5 12.3 5.3 2.0 1.5 4.0 0.2 0.7 0.7 0.3
Note: Values quoted are the average of five area analyses by SEM-EDS on different areas of the sample.
92 HM 44(2) 2010 ANGUILANO ET AL: LEAD SMELTING AT CWMYSTWYTH
Figure 7: Optical image of slag sample 5-4a showing glassy Figure 8: Optical image of slag sample 6B-2b-f showing the matrix (dark) and residual galena (light grey) with typical glassy matrix (darker grey), silicates (paler grey) and crystalline triangular cleavage pattern. Image width 500µm. sulphides (white). Image width 200µm. minerals: the only trace of high temperature processes are scatter of newly-formed opaque crystals with a spherical erosion bays where the slag is in direct contact with the or dendritic shape, tentatively identified as lead sulphide. rock. The bulk composition of one sample of furnace wall The volume proportion of lead sulphide varies within had been determined by XRF (Table 3). The silica:alumina and between samples from a few percent to eight or ratio is 5:1, calcium and magnesium oxide are less than ten percent. In some of the samples, long needle-like 1% and the sum of sodium and potassium oxides is less or skeletal silicate crystals were identified. There was than 4%. The lead oxide content of 4% indicates some no intergrowth between sulphides and silicates, both of contamination by adhering slag in this sample. them formed separately in the glassy matrix.
The three unreacted ore samples (eg Fig 6) are The main oxide concentrations in the slag samples as mineralogical associations of galena with quartz in dif- analysed by ED-XRF are shown in Table 2. The slag is ferent concentrations (from thirty to just a few percent of dominated by lead oxide (c70wt%) and silica (c15–20- quartz) and they present the typical triangular cleavage wt%) with minor amounts of alumina, zinc and iron ox- pattern of galena. At least one of the galena samples is ides. Remarkable is the high sulphur content of c3–4wt%. also associated with glassy slag, indicating that these ore The bulk analyses confirm the overall homogeneous samples were directly exposed to the smelting process composition of the slags. The ‘metallic’ component of although they obviously did not react fully. Conversely, the slag is dominated by the association lead-zinc with it is possible to see re-crystallized galena within the rather low iron oxide, suggesting an ore association of glass, and reaction bays between galena and glass (Fig 7) galena-sphalerite with only a minor amount of pyrite. representing more advanced but still incomplete stages The almost complete absence of copper (below c0.01% of the reaction. in all analyses) suggests the absence of chalcopyrite from the smelting charge. Noteworthy is the low con- Only some of the micro-analyses of the galena sample centration of typical rock components other than silica, (6B-2b-g) showed a local concentration of silver around which suggests a charge comprising almost exclusively 0.2wt%, others failed to detect silver altogether (the of galena plus quartz. silver detection limit in EDS is 0.1%) agreeing with the bulk concentration of silver of around 10ppm measured To further test the possible contribution of furnace wall by XRF (Table 2). No silver was detected in the SEM- material to slag formation, the ratio of SiO2:Al2O3 in the EDS area analysis of the metallic lead associated with two materials were compared. In the slag it is between the slag sample 6B-2b-c, and only less than c470ppm 10:1 and 15:1, while in the furnace wall it is only about during the bulk analyses of either galena or lead metal 5:1. Obviously there is only a limited contribution of by ED-XRF. alumina to the slag, resulting from the aggressiveness of lead oxide during the smelting against the wall. The The slag samples are petrographically all rather homo- most likely origin of this concentration of silica in the geneous (Fig 8). The matrix is completely glassy with a slag is the presence of quartz with the galena during the
93 ANGUILANO ET AL: LEAD SMELTING AT CWMYSTWYTH HM 44(2) 2010
Figure 10: Silica (SiO2) and lead oxide (PbO) content of the Figure 9: Silica (SiO2) and lead oxide (PbO) content of the slag glassy matrix of the slag samples from Banc Tynddol (SEM- samples from Banc Tynddol (XRF analyses). EDX analyses). smelting. It has to be discussed whether the quartz was During the SEM-EDS analyses different types of slag added on purpose as a flux, or whether it represents un- were identified based on their population of silicate intentional gangue from the ore. Noteworthy also is the crystals. Some had a fully-glassy matrix, some showed very low concentration of calcium and barium oxide in a scatter of silicate crystals seemingly floating freely in the slag, in stark contrast to the majority of bale slags the predominantly glassy matrix, and one sample was from medieval Yorkshire (Smith and Murphy, this vol- completely crystalline. The latter sample showed a char- ume) reflecting the very different gangue composition acteristic spinifex texture; the crystals are thin and skeletal of the ores from the two regions. with growth orientation perpendicular to the cooling sur- face. A further distinction within the crystal-containing The SEM-EDS analyses of the glassy or microcrystalline slags is based on the different types of silicates present. part of the slag (Table 1) confirmed in principle the XRF One type can be described as Pb4(Al6Si20)O53 (sample data. However, sulphur is below the detection limit, 5-4c; Fig 11), another as PbZnSiO4, (samples 6B-2b-a the lead levels are slightly lower and the other oxides and 6B 5-4e ), and the third one (6B-2b-d), showing the accordingly increased, reflecting the exclusion of the spinifex texture and forming a fully crystalline matrix lead sulphide crystals from the analyses (Figs 9 and 10). (Fig 12), has a formula similar to PbSiO3. The differences may also reflect different calibration and evaluation procedures for the two different instruments, The fully crystalline sample is compositionally no as mentioned above. different from the majority of the other samples; its
Figure 11: Secondary electron image of sample 5-4c showing the Figure 12: Secondary electron image of sample 6B-2b-d showing glassy matrix (light grey) and associated alumina-silicates (dark sulphides (light) associated with fully crystalline spinifex matrix grey) and sulphides (white). Image width 200µm. (two tones of mid grey). Image width 100µm.
94 HM 44(2) 2010 ANGUILANO ET AL: LEAD SMELTING AT CWMYSTWYTH
Figure 14: BSE image of slag sample 6B-2b-c showing lead Figure 13: Zinc oxide (ZnO) and lead oxide (PbO) content of metal (pale grey with black spots) segregating from lead sulphide the glassy matrix of the slag samples from Banc Tynddol (SEM- (light grey). Image width 200µm. EDX analyses). different structure probably reflects a slightly slower cooling history, with more time enabling crystal nu- cleation and growth. However, the cooling still took place relatively rapidly as indicated by the spinifex structure. The sample comprising the alumino-silicate crystals has overall higher alumina and silica levels in the glass phase than the other slag samples, and accord- ingly a lower lead oxide concentration. However, it is not fundamentally different from the other slags, and may simply represent a composition with a slightly higher contribution of absorbed furnace wall material and a richer concentration of residual quartz. Similarly, the two samples with lead-zinc silicates show no appar- ent compositional peculiarity which would explain the Figure 15: BSE image of slag sample 6B-2b-c showing lead presence of these crystals, so we assume that only slight metal (with-grey with black spots) segregating from lead sulphide variations in nucleation and cooling history resulted in (light grey). Image width 200µm. the growth of these crystals here.
Figure 13 shows the ratios between ZnO and PbO in the diffusion of the elements and the temperature. glass matrix, in particular the distinction of the sample 6B-2b-d which has the lowest concentration of zinc in SEM-EDS analyses of the sulphides invariably con- the glass matrix but is also the only one that contains firmed their optical identification as lead sulphide (PbS) zinc in the sulphides. Sample 5-4c contains zinc only in with an almost stochiometric composition of c13wt% S the glass matrix and is the lowest in PbO. The peculiarity and c86wt% Pb. In all the samples larger areas of lead of sample 5-4c is mainly linked to the high silica (and sulphide are visible, forming matte inclusions with alumina) content (Fig 10); this high concentration affects segregation of lead metal (Figs 14 and 15); these are the concentration of PbO, which is therefore lower in apparently formed from the melt rather than being this sample. Sample 6B-2b-d does not have complete residual or re-crystallized galena. They indicate that the decomposition of the sulphides, so we can still note system, even when at a sufficiently high temperature some zinc in them, while the liquidus phase (the glass) to be fully liquid, was still so rich in sulphur to allow is not as enriched in zinc as the other analysed samples. only part of the lead to be present as metal, while some These small differences between the samples, discussed was still forming a separate lead sulphide phase due to below, are probably connected to the heterogeneity of incomplete reaction of the charge. the system in the furnace, regarding both the chemical
95 ANGUILANO ET AL: LEAD SMELTING AT CWMYSTWYTH HM 44(2) 2010
from the melt. The relatively low level of other ore- related oxides, such as zinc, iron or copper, indicates that the ore was almost pure galena.
The high silica:alumina ratio in the slag, of about 15:1, shows that contamination of the slag from the furnace wall played only a very minor role, otherwise higher alumina levels would be expected in the slag. This indicates that the silica in the slag originates predominantly from the quartz gangue of the charge. The analyses of the glass matrix show the composition of the liquid phase during the pro-
cess. It is interesting to compare the SiO2-PbO data in the glass (Fig 16), which are consistent with the bulk data, with
the SiO2-PbO phase diagram (Geller et al 1934). The data Figure 16: Optical image of slag sample 6B-2b-f showing the show firstly that the minimum temperature of the process glassy matrix (darker grey) and crystalline silicates (pale grey) was around 750°C. The composition is mainly at the top and sulphides (white). Image width 500µm. of the cotectic curve (~760°C) joining the eutectics at 15
and 30% SiO2, except for sample 5-4c whose composition
is close to the eutectic richer in SiO2 (~740°C). These Interpretation and discussion temperatures are for the pure system SiO2-PbO but the The ore smelted was predominantly galena with quartz presence of several minor oxides is likely to reduce these gangue; some sphalerite and minor pyrite were also temperatures further. The peculiarities of sample 5-4c are present, as indicated by small concentrations of zinc an example of the heterogeneity of the conditions inside and iron in the slags. The complete absence of carbon- the furnace, for the composition of the charge, the role of ate gangue and chalcopyrite would seem to reduce the the furnace lining for the material closer to the furnace likelihood that the ore was obtained nearby, either from wall, and for the temperature inside the furnace. The other the Comet or Penguelan mineral lodes at the foot of Copa point is that at this temperature (~750°C ) the slag could Hill (Hughes 1981; Timberlake 2003). Instead the most have absorbed more silica than it did solidifying following probable near-surface source is the Kingside Lode on the the cotectic line and ending up with a solid at the eutectic at Graig Fawr or where this has been worked by old surface 30% silica. This could indicate that the addition of quartz rakes on the northwest slopes of Copa Hill (ST). was not deliberate, the material smelted was simply the ore including the average of gangue already associated with Noteworthy are the rather low overall silver levels found it; and that the medieval lead smelters knew that their raw in ore, slag and metal. They do not exceed a few hundred material was pure enough not to need a further addition of ppm, and would therefore not have been economically quartz. On the other hand, this makes the slag aggressive viable to extract during the Middle Ages. Rehren and against the siliceous stones from which the furnace was Prange (1998) discussed economic cut-off grades for built, as can be seen in the erosion cavities at the interface silver levels in Late Bronze Age and Roman lead, and between slag and furnace wall, and the limited uptake of found that silver extraction in these periods is not alumina into the slag. economical below about 600–1000ppm. No comparable data exist for the medieval period; however, it is unlikely The combination of limited silica in the charge, the that the cut-off grades would have been significantly highly sulphuric conditions in the furnace and the lower as early-medieval technology was no more ad- relatively low temperatures make this an interesting vanced than Roman technology, and large amounts of model for a well-balanced furnace operation. This can silver from Central Asia flowed into northern Europe via be considered a technical choice in order to limit the the Viking trade prior to the 10th century AD. production of slags while maintaining a non-oxidiz- ing atmosphere, which limits the formation of lead The very high sulphur content of the slag (around 3wt% silicates. Pre-roasting of the ore could have resulted compared to the 0.05wt% average indicated for fayalitic in higher formation of lead oxide, which would be slags of the same period by Tylecote (1987, 302)) more aggressive towards the furnace wall rather than indicates that the ore was not roasted before smelting, increasing the yield through reduction to lead metal. resulting in only partial reduction of some of the metal, Allowing lead sulphide to form as an excess phase is and the abundant precipitation of lead sulphide crystals in contrast less deleterious, and any matte recovered
96 HM 44(2) 2010 ANGUILANO ET AL: LEAD SMELTING AT CWMYSTWYTH from the slag could easily have been reprocessed with in 2005). At 800°C the reaction between lead oxide and the next smelt, together with fresh galena. This choice lead sulphide is possible (Tylecote 1987, 112) without could also be connected with the need for saving fuel the need of a more complex furnace. In the case of Banc for the process in one area where the easy availability Tynddol, in this central area of the furnace the reaction of the pure raw material allows the waste of part of the between the oxidized lead and the residual galena or the metal as matte. new-formed matte might have happened at a temperature as high as 1200°C, depending on the size of the furnace. How does this slag compare with lead slag from other Of course we have to bear in mind that this furnace is an sites? The overall composition of the slag differs sig- open structure completely dominated by the wind action. nificantly from the other known medieval lead smelting In the same experiment carried out in 2005, a difference sites, indicating a different smelting technology. Murphy in temperature in the furnace of 200°C was noticed with (1992) identified three different types of remains from a change of only 1m/s in the wind’s speed. ore hearths:white-coated material, dark-grey black slag and vitreous black slag. The content of lead in those slags With very pure raw materials, the only slags formed are the varies from 12wt% in the glassy black slag to 17wt% in ones connected with the presence of quartz and the other the dark-grey slag. Both of these are far lower than the few impurities (as Zn and Fe) coming from the charge, and concentration of lead in Banc Tynddol slag (≈ 65–70wt% the impurities coming from the degradation of the furnace PbO, Table 3). Other lead-rich slags mentioned in the walls due to the aggressiveness of lead oxide. It looks as if literature are from Pentre Ffwrndan (Wales) with around a small amount of quartz was left in the charge, possibly 30wt% lead oxide (Atkinson et al 1924–5) and the consciously, in order to help purify completely the already Pennines, with around 50wt% (Tylecote 1987); still much fairly pure and massive galena ore, accepting some waste less than the 65–70wt% found in the slags from Banc of part of the lead in order to absorb the minor amounts of Tynddol. The slags from the Pennines are identified as zinc and iron present within the ore. remains of a bole smelting process needing a further step in a slag hearth, while the slags from Banc Tynddol are the The furnaces used apparently did not require much result of a one-step process in a hearth furnace. For Banc capital investment, enabling a short-lived and/or ex- Tynddol, one can further discuss the slag composition in ploratory-like smelting operation to be conducted. view of the quantities found during the excavation, and the The absence of silver within the lead sample analysed nature of the furnace installations unearthed. The amount suggests to us that the galena was not exploited to pro- of slag is rather low, so that even if it is lead rich, it will cess the lead in order to obtain silver, but only to obtain still not represent a major loss in metal. Furthermore, lead itself. However, we still cannot say with confidence the furnace excavated is a simple and low-cost structure, whether smelting was carried out here on a regular basis made of local stones, and most probably wind-blown, to produce small quantities of lead metal, or whether compatible with a low-key operation. these were just test smelts in order to assess the quality of the ore and to assay it as a potential source of silver. Conclusions It is argued that the medieval activity at the site was The experimental reconstruction and small-scale, smelting a very rich lead ore under con- operation of a medieval bole hearth at ditions which limited the amount of slag produced while Penguelan, Cwmystwyth (ST) at the same time tolerating a rather lead-rich slag. In May 2003, one of the authors (ST) carried out an Considering the remains analysed, the results obtained experimental lead smelt within a dry stone-walled bole and the description of a leadsmelting process by Tylecote hearth constructed on a patch of high ground located (1987, 112) we get the image of a hearth furnace, with on the flattened tips of the old Penguelan Mine, just a footprint of about one square metre, completely filled above the Banc Tynddol meadow and some 25m north with wood, maybe mixed with charcoal, with different of the excavated medieval hearth in PSS 6 (Fig 2c). layers of charge in it, but mainly on the surface. When the The experiment tried to reconstruct the sort of hearth temperature is high enough (around 300°C) the oxidation which might have been in use at the latter site during reaction (the roasting) would start and the semi-reacted the early-medieval period. The intention was to observe material would begin sinking into the furnace, where the the progress and conditions of the smelt and to collect temperature would easily reach 800°C in around two and analyse the smelt products. hours with a wind speed of between 4 to 5m/s (based on an experiment carried out by LA on Banc Tynddol Although detailed analysis of these smelt products has
97 ANGUILANO ET AL: LEAD SMELTING AT CWMYSTWYTH HM 44(2) 2010
Figure 17: The experimental bole hearth. a) diagrammatic cross-section before burning; b) plan after smelting. b
not yet been undertaken, much information could be Derbyshire boles such as the Totley Bole Hill (Kiernan gleaned from recording the process in action and also and Van de Noort 1992) and from the excavation record from a visual inspection of the partially-smelted ore and of the medieval bole dug at Beeley, Derbyshire in 1967. lead metal afterwards. These findings were something of The latter had been built into the structure of a triple a revelation to our understanding of the process. Bronze Age cairn (Radley 1970).
The smelt was carried out over a period of three hours The walls of the Penguelan bole were constructed of flat on the evening of the 15th May, the significant limiting riverine boulders plus shale and quartz mine waste, and factor here being the amount of dry, chopped firewood as with the hearth sites found in the excavations in area which could be contained within a much scaled-down PSS6 this was constructed directly on top of the turf, walled hearth, and also the small amount of hand-picked without any sort of scooped-out base or hollow under- galena available to us, all of the latter collected within neath. The external dimensions were about 1.5m by 1.2m a 500m radius of the site. wide and 0.7m tall, but internally this was no more than 0.65m by 0.45m wide, a space which was compactly The design of the sub-circular dry stone-walled bole stacked to a height of only about 0.35m with split wood structure was loosely based upon the evidence un- (cord wood) and layers of crushed ore (Fig 17a). Built covered during the excavation of PSS6, as well as from into the base of the walling surround on both east and historical record and field remains of post-medieval west sides of the hearth were small openings or ‘wind
98 HM 44(2) 2010 ANGUILANO ET AL: LEAD SMELTING AT CWMYSTWYTH arches’ and in addition funnel-like projections beyond round, whilst a yellowish deposit (lead oxide) could be in the form of two pairs of low stone walls some 1–2m seen on some of the burnt wood around the edges of the long converging on each of the openings. The latter fire. Although no accurate record of the temperatures would act as funnels or wind-tunnels to concentrate the reached inside of the hearth was taken, at this point it action of the prevailing winds and help raise the smelting was estimated to be around 750–800°C based on visual temperature within the hearth (these winds were mostly colorimetry of the still-burning embers and mass of westerly channelled up the Ystwyth Valley from the fused/molten ore lying within the base of the bole. One coast some 20km away). Such a careful arrangement and half hours later these embers were still burning, of ‘wind gathering’ is recorded at Beeley (Radley 1970) fanned by a light, steady breeze, but by 9pm this had although of course nothing at all has survived of any died down and nearly ceased altogether; the smelting of these above-ground walled structures within the process was probably now at a halt, frozen as the light Banc Tynddol excavations. Thus while the use of wind patter of rain increased, and the wind died. funnels is known about, the actual lay-out of the bole construction at Penguelan was little more than calculated The results of the smelting were examined the follow- guesswork based on the excavator’s own judgement of ing morning, the overnight rain having washed out the the topography and wind dynamics of the site. tops of the embers, exposing part-fused galena lumps lying above the burnt clay ground surface (Figs 17b and The experimental hearth was tightly packed with some front cover). The formerly soot-blackened rock of the 74kg of wood composed of alternate cross-wise layers of stone-walled hearth surround was now fire-reddened, split 200–300mm by 60–80mm logs of ash and Douglas and the white deposit visible the day before coating the fir (chosen because of its hot-burning properties) plus surfaces of the stones more or less invisible, the latter brushwood kindling, with all of the thicker and more perhaps washed away or else still further altered. On tightly-packed and un-split large logs stacked at the the northeast side of the hearth a deposit of metallic base, an arrangement similar to that found within the dust (lead?) had formed on one of the stones on top of excavated hearth at Beeley, and believed there to have the walled surround, while small amounts of galena been an attempt to prevent the heavy ore sinking too dust ‘blown out’ by the force of the combustion or else quickly into the base before being oxidized (Blanchard by the squalls of wind lay scattered over the ground 1992, 11). Interleaved, in amongst the wood, were some outside the hearth. Flakes of rock ‘spalled-off’ by the 2–3 layers of crushed galena, most of this in ‘hazel nut’ heat of the fire from the stones lining the inside of the to ‘walnut-sized’ pieces (of a similar size fraction to that hearth wall covered much of the interior of the bole. In recovered from Banc Tynddol (Fig 18)), hand-picked both size and appearance these matched well the type and wherever possible separated from most of the ad- of burnt rock fragments found in layer 006b within area hering blende and larger pieces of quartz and carbonate PSS6 of the Banc Tynddol excavations. The latter had gangue. In total the ore charge amounted to some 8.5kg been found covering the charcoal and ancient burnt of galena, a ratio of about 1:10 of ore to fuel. turf horizon exposed within the area of the medieval smelting hearth. Many of the rock fragments from the The experimental smelt commenced about 6pm (see experimental smelt showed some evidence of surface front cover for its progress) the bole being lit from the vitrification in the form of brown-green slaggy glazing base, with the bulk of the wood quickly catching fire (lead silicate), some of this being fused together in the and burning strongly fanned by a variable but strong fire. Immediately beneath the centre of the hearth a breeze . At the end of the first 20–25 minutes yellow sul- patch of burnt earth indicated the area of greatest heat phurous fumes (sulphur dioxide) within the smoke plume penetration, whilst just above this was found a large indicated an effective roasting of the ore, and some of mass of partly fused and smelted lead ore. However, these gases were collected for analysis. After 6.30pm the the largest single concentration of lead metal droplets, breeze increased to small gusts, predominantly from the some joined with pieces of incompletely smelted galena west, but thereafter this changed to intermittently west in a network of lead metal runnel, was to be found out- and east squalls, resulting in some swirling effect of the side of this central zone, closer to the hearth wall and fire around the base of the bole site, but not diminishing in particular to the eastern ‘wind arch’ situated on one the rate of combustion. By 6.55pm the wind had died side of the furnace. down considerably, but by this time much of the wood had already burnt down. On approaching the bole, a Effectively the smelting process we had witnessed here white-blue sublimate deposit (zinc oxide) was noticed was incomplete. The smelt seems to have been frozen on the side of some of the boulders in the walling sur- in mid-flight, perhaps due to the exhaustion of the fuel,
99 ANGUILANO ET AL: LEAD SMELTING AT CWMYSTWYTH HM 44(2) 2010
covered appears similar in some ways to that of melted chocolate (Fig 19), whilst in some pieces this process was rather more advanced, as can be seen in the frag- ment drawn in Figure 20. Here the original lump of ore appears, literally, to have shrunk and collapsed, leaving the gangue impurities on the exterior with a long runnel of lead metal emanating from it.
All of these fragments of lead metal and part-smelted and un-smelted ore were collected, examined and weighed. Some 150g of the total mass appear to be discreet identifiable droplets, runnels and amorphous lumps of Figure 18: Typical ore charge, a crushed fragment of rich hand-picked galena. Scale 50mm. pure lead metal, the remaining 8kg being incompletely smelted ore with minor amounts of lead metal attached alongside adhering lead ‘slag’ and charcoal. No lead-rich a cessation of the breeze and consequent plummeting glassy slags similar to those recovered from the medieval in the furnace temperature, but also to changes in the hearths in area PSS6 appear to be present, not surpris- oxidizing/reducing conditions prevalent within the ing in view of the much lower temperatures and only hearth. However, what we can see on close study of poorly-reducing conditions achieved. However, some those part-smelted galena lumps examined (Fig 18) interesting insights into the process had been achieved, is that there is some evidence for localized oxidation and some useful parallels could now be drawn. and reduction and then melting and coalescence of the metal into droplets on the external surfaces of the ore Conclusions pieces. This could also be seen happening in real time The achievement of an ‘unsuccessful’ smelt has in some as the fire died down, and is recorded in some of the ways been much more useful to us than if it had all photographs taken looking down into the centre of the gone well and we had been left with a separated pool hearth. These show lead metal forming like beads of of lead metal and ‘slags’. Being able to observe the silvery solder on the outside of the red-hot glowing process ‘frozen’ in mid-smelt afforded us a rare insight lumps of ore. As the smelting progressed these drops into the way the metal forms and the way it is liberated appear to have been gathering into incipient runnels from the ore (at least under these poorly-reducing and prior to any proper pooling of the metal. The latter does relatively uncontrolled smelting conditions). In effect not appear to have taken place, probably on account of the smelting appears as a one-step process of virtually the fire having burnt down and the resultant temperature simultaneous oxidation and reduction from sulphide to drop. The external texture of many of the ore pieces re- metal without any oxide stage being visible. This con-
Figure 19: Part smelted and fused galena coated with lead metal droplets and impression(s) of burnt wood. Scale 50mm
100 HM 44(2) 2010 ANGUILANO ET AL: LEAD SMELTING AT CWMYSTWYTH
At Banc Tynddol the presence of a significant amount of cobbled and only part-smelted galena also attests to a problem of insufficient temperature and/or duration of smelting within some parts of the bole pile, and in that respect at least the similarity of the experimental hearth reconstruction to whatever sort of bole structure may have been in use during the early-medieval period is probably close. Moreover, there seems little doubt that the dynamics and efficiency of these boles would always have been difficult to control, particularly when subject to the vagaries of wind and changeable weather. Nevertheless, careful choice of weather conditions, for example choosing a period which was experiencing a series of constant, prevailing, and dry winds (such as one might occasionally find in May/June or September/ October) might considerably aid the efficiency of the smelt and yield. This is just the sort of area that now requires a considerable amount of experimental Figure 20: Almost fully-smelted galena, the original ore lump investigation, and one for which historical records have has collapsed and has a runnel of lead metal emanating from it. Scale 50mm. so far yielded little.
With respect to the wind effect it was therefore par- firms the interpretation offered for the process of bole ticularly interesting to find that the greatest production smelting described from the medieval hearth at Beeley of lead metal within the experimental hearth occurred in Derbyshire (Blanchard 1992, 11), with the oxide around the margins of the bole closest to the two ‘wind reacting directly with the un-roasted ore as shown in arches’, in particular the eastern opening. This may the following equations: suggest that smelting was most effective at the interface oxidation: of the most oxidizing and reducing conditions within the
PbS+2O2 = PbSO4 and/or furnace. Furthermore the much smaller galena fragments
2PbS+2O2 = 2PbO+SO2 do not appear to have undergone smelting any more followed by simultaneous reduction: effectively than the larger ‘walnut-sized’ pieces. In fact,
PbS+PbSO4 = 2PbS+2O2 and/or the evidence we had suggested that the ideal size of ore
2PbO+PbS = 3Pb+SO2 particle for smelting under these conditions was about 10–20mm (‘hazel nut’ size), something supported also One wonders whether under more oxidizing conditions, perhaps by the archaeological evidence from area PSS6 but with sufficient fuel and duration of smelt, these at Banc Tynddol where this size of cobbled ore fragment primitive boles might actually have been more efficient. is commonly found both underneath and around the site Where too-reducing conditions are met with in parts of of the former hearths. the hearth, lead sulphide will re-form, whilst too hot and reducing conditions may result in the deposition of eutectic There are many individual variables which need to be lead-glass slags, resulting in an overall loss in lead metal tested in future experiments, including the dimension of yield. The latter seems to have taken place, to a greater or boles, the quantities and ratio of ore to fuel, the methods lesser extent, within the medieval boles excavated at Banc of stacking, the type of walled hearth surround, the Tynddol, though here the presence of such slags might presence or absence of ‘wind arch’ openings and funnels, just represent the outcome of one or more unsuccessful and of course the all-important factors of wind speed, smelts within a sequence, or a minor part of an otherwise wind constancy, temperature and dryness. Continuous successful smelt and yield of metal, or else an attempt at monitoring of the latter during the smelting alongside re-smelting lead slags gathered from elsewhere. Larger a record of the various temperature(s) reached within boles may proportionately have produced rather more slag different parts of the bole stack would be a very useful and also experienced much greater lead loss, yet overall aid to understanding the factors affecting the success these would probably still have been more efficient on fuel of the smelt and the efficiency of lead yield. Clearly relative to the amount of lead metal produced. ‘freezing’ the smelt at different stages in its progress can help us to understand the process a good deal better. One
101 ANGUILANO ET AL: LEAD SMELTING AT CWMYSTWYTH HM 44(2) 2010 way to do this would be to rake out the burning hearth memory of David Bick (1930–2006). Over the last 20 or possibly to quench it. Needless to say, there are im- years of his life David gave his wholehearted supported portant health and safety considerations to address in to these sorts of investigations into early mining and trying to attempt this! smelting in Wales, on many occasions helping to fund archaeological work out of his own pocket. Our subject Opportunities available today to carry out such experi- is all the richer for it. ments on lead furnaces in the open together with the permission of landowners and statutory conservation References bodies are becoming rarer and rarer. In this respect we have been very fortunate, although there are of course Atkinson D, Petch, J A and Taylor, M V 1924–5, Flint Excavation risks inherent in carrying out the work, in particular Reports, Flintshire Historical Society Publications X (1924–5) Parts 1 and 2 conducting close-up photography during the smelting Blanchard I 1992, ‘Technical implications of the transition from process. Partly for this reason the boles have been kept silver to lead smelting in twelfth century England’, in L Willies small and their operation limited to just one or two and D Cranstone (eds), Boles and smeltmills (Matlock Bath: people at a time. It would certainly be desirable now to Historical Metallurgy Society Occasional Publication 3), 9–12. repeat the above process exactly, using the same amount Chambers W 1858, ‘Letter from Hafod, July 29’, Mining Journal [for 1858], 513. of ore but with slightly more fuel, and carried out under Davies O 1936, ‘Early Mining Sites in Wales’, Report Annual much more constant wind conditions. Meeting British Association for the Advancement of Science, Section H, 304–305. Davies O 1937, ‘Early Mining Sites in Wales’, Report Annual Acknowledgments Meeting British Association for the Advancement of Science, Section H4, 301–303. Dobson M R 1995, ‘The Aberystwyth District’, Geologists’ The costs of excavation and post-excavation work Association Guide No 54 (London), 89–91. carried out by the Early Mines Research Group at Banc Geller R F, Creamer A S and Bunting E N 1934, ‘Research Paper Tynddol in 1999 and 2002 were grant-assisted by the No RP 705’, Journal of Research of the National Bureau of Standards, 13, 237–244. Cambrian Archaeological Association and the Board Hughes S J S H 1981, The Cwmystwyth Mines (Sheffield: British of Celtic Studies (2002). The National Museum and Mining 17). Galleries of Wales helped fund further work in 2003 Hughes S J S H 1990, The Darren Mines (Sheffield: British Mining along with the costs of radiocarbon dating. Mrs M Raw 40). of Ty Llwyd Farm gave permission for the work whilst Jenkins D and Timberlake S 1997, ‘Geoarchaeological research into prehistoric mining for copper in Wales’. Unpublished report to scheduled monument consent was provided by CADW. the Leverhulme Trust, University of Wales, Bangor. Geochemical survey work was carried out with the help Jones O T 1921, Lead and zinc: the mining district of north of David Jenkins and Andy Owen (formerly at Bangor Cardiganshire and west Montgomeryshire. Memoirs of the University) whilst the geophysical surveys were under- Geological Survey: Special reports on the mineral resources of taken in 1999 by Martin Roseveare of Archaeophysica Great Britain 20 (London). Kiernan D and Van de Noort R 1992, ‘Bole smelting in Derbyshire’, Ltd. The late David Bick and also George Hall (of the in L Willies and D Cranstone (eds), Boles and smeltmills (Matlock Welsh Mines Society) passed on information concern- Bath: Historical Metallurgy Society Occasional Publication 3), ing the Hafod bole site, as did Peter Claughton on the 19–21. history of bole smelting. Brenda Craddock (EMRG) has Lewis 1967 Lead Mining in Wales (Cardiff). Meyrick S R 1907, The history and antiquities of the county of carried out most of the illustration work (Figures 1, 2c, Cardiganshire (Brecon). 17, 18–20). Our particular thanks go to Barry Clarke who Mighall T M, Timberlake S, Grattan J P and Forsyth S 2000, ‘Bronze provided the main assistance during the experimental Age lead mining at Copa Hill, Cwmystwyth—fact or fantasy?’, bole smelt in 2003. Historical Metallurgy 34(1), 1–12. Mighall T M, Grattan J P, Lees J A, Timberlake S and Forsyth S 2002, ‘An atmospheric pollution history for Pb-Zn mining in The analyses were done at the Wolfson Archaeological the Ystwyth Valley, Dyfed, mid-Wales, UK’, Geochemistry: Science Laboratories at the Institute of Archaeology, Exploration, Environment, Analysis 2, 175–184. UCL, with the co-operation of Simon Groom (XRF Murphy S 1992, ‘Smelting residues from boles and simple smeltmills’, laboratory supervisor) and Kevin Reeves (SEM laboratory in L Willies and D Cranstone (eds), Boles and smeltmills (Matlock supervisor), funded by the European Union under a Bath: Historical Metallurgy Society Occasional Publication 3), 43–47. Marie Curie Host Fellowship for Early Stage Researchers Radley J 1970, ‘A triple cairn and a rectangular cairn of the Bronze Training, contract MEST-CT-2004-514509. Age on Beeley Moor’, Derbyshire Archaeological Journal 89, 1–17. The authors would like to dedicate this paper to the Rehren T and Prange M 1998, ‘Lead metal and patina: a comparison’,
102 HM 44(2) 2010 ANGUILANO ET AL: LEAD SMELTING AT CWMYSTWYTH
in T Rehren, A Hauptmann and J Muhly (eds), Metallurgica at the Institute of Archaeology, UCL on jarosite exploitation and Antiqua, in honour of Hans-Gert Bachmann and Robert Maddin silver production at Rio Tinto, Spain. She is currently research (Bochum: Der Anschnitt Beiheft 8), 183–196. Timberlake S 1990, ‘Excavations and Fieldwork on Copa Hill, fellow for the application of X-ray techniques to material science Cwmystwyth, 1989’, in P Crew and S Crew (eds), Early mining at Brunel University. in the British Isles (Plas Tan y Bwlch), 22–29. Address: Experimental Technique Centre, Brunel Timberlake S 2002a, ‘Cwmystwyth, Banc Tynddol (gold disc)’, University, Kingston Lane, Uxbridge UB8 3PH. Archaeology in Wales 42, 97–98. e-mail: [email protected] Timberlake S 2002b, ‘Medieval lead-smelting boles near Penguelan, Cwmystwyth, Ceredigion’, Archaeology in Wales 42, 45–59. Timberlake S 2003, Excavations on Copa Hill, Cwmystwyth (1986- Simon Timberlake has undertaken research at sites 1999): An Early Bronze Age copper mine within the uplands of of early mining in mid-Wales and elsewhere. He has Central Wales (Oxford: British Archaeological Reports, British worked at Bangor, Manchester and Coventry Universities Series 348). on early mining-related research projects funded Timberlake S 2004, ‘Cwmystwyth, Banc Tynddol (grave and Beaker gold disc)’, Archaeology in Wales 44, 137–139. by the Leverhulme Trust and joined the Cambridge Timberlake S 2009, ‘Copper Mining and metal production at the Archaeological Unit in 2006. He is interested in experi- beginning of the British Bronze Age’, in P Clark (ed), Bronze mental archaeology and the reconstruction of prehistoric Age connections: cultural contact in prehistoric Europe (Oxford), mining and smelting processes, and has published many 95–122. Tylecote R F 1986, The prehistory of metallurgy in the British Isles papers on early mining. (London). Address: 13 High Street, Fen Ditton Cambridge CB5 Tylecote R F 1987, The early history of metallurgy in Europe 8ST. (London). e-mail: [email protected] Williams S W 1889, The Cistercian abbey of Strata Florida: its history, and an account of the recent excavations (London). Willies L and Cranstone D (eds) 1992, Boles and smeltmills (Matlock Thilo Rehren’s interests lie in reconstructing and Bath: Historical Metallurgy Society Occasional Publication 3). understanding high-temperature processes used in the production of metals, glass and glazes. He has worked on materials from all over the world; his current pro- jects are diverse, ranging from Europe to China to The authors South America. From 1999 to 2011 he was Professor for Archaeological Materials and Technologies at UCL Lorna Anguilano started her archaeometallurgical career in 2000 Institute of Archaeology, and recently became Director reconstructing the different processes of copper production in of UCL-Q in Doha, Qatar. the Middle and Late Bronze Age in the South Tyrol. In 2003 Address: PO Box 23689, Georgetown Building, she started working on lead and lead/silver production with two Education City, Doha, Qatar. projects in Wales and Greece. She recently completed her PhD e-mail: [email protected]